of Chemical Composition9
E 213 Practice for Ultrasonic Examination of Metal Pipe
E 309 Practice for Eddy-Current Examination of Steel Tu-
bular Products Using Magnetic Saturation10
E 570 Practice for Flux Leakage Examination of Ferromag-
netic Steel Tubular Products10
2.2 ANSI Standards:
B1.20.1 Pipe Threads, General Purpose11
2.3 ASME Standard:
B36.10 Welded and Seamless Wrought Steel Pipe12
2.4 Military Standards:
MIL-STD-129 Marking for Shipment and Storage13
MIL-STD-163 Steel Mill Products Preparation for Ship-
ment and Storage13
2.5 Federal Standards:
Fed. Std. No. 123 Marking for Shipment (Civil Agencies)14
Fed. Std. No 183 Continuous Identiﬁcation Marking of Iron
and Steel Products14
2.6 API Standard:
5L Speciﬁcation for Line Pipe15
3. Ordering Information
3.1 Information items to be considered, if appropriate, for
inclusion in the purchase order are as follows:
3.1.1 Speciﬁcation designation (A 53 or A 53M, including
year of issue),
3.1.2 Quantity (feet, metres, or number of lengths),
3.1.3 Grade (see Table 1),
3.1.4 Type (see 1.2 and Table 2),
3.1.5 Finish (black or galvanized),
3.1.6 Size (either nominal (NPS) [DN] and weight class or
schedule number, or both; or outside diameter and nominal
wall thickness, Table X2.2 and Table X2.3),
3.1.7 Length (speciﬁc or random, Section 18),
3.1.8 End ﬁnish (plain end or threaded, Section 13),
188.8.131.52 Threaded and coupled, if desired,
184.108.40.206 Threads only (no couplings), if desired,
220.127.116.11 Plain end, if desired,
18.104.22.168 Couplings power tight, if desired,
22.214.171.124 Taper tapped couplings for NPS 2 [DN 50] and
smaller, if desired,
3.1.9 Close coiling, if required (see 8.2),
3.1.10 Skelp for tension tests, if permitted (see 17.2),
3.1.11 Certiﬁcation (see Section 22),
3.1.12 End use of material,
3.1.13 Special requirements, and
Discontinued 1996; Replaced by E 1806.
Annual Book of ASTM Standards, Vol 03.03.
Available from American National Standards Institute, 11 West 42nd St., 13th
Floor, New York, NY 10036.
Available from ASME International, Three Park Avenue, New York, NY
Available from Standardization Documents Order Desk, Bldg. 4 Section D,
700 Robbins Ave., Philadelphia, PA 19111-5094, Attn: NPODS.
Available from General Services Administration, Washington, DC 20405.
Available from American Petroleum Institute, 1220 L Street, Northwest,
Washington, DC 20005–4070.
TABLE 1 Chemical Requirements
Composition, max, %
Carbon Manganese Phosphorus Sulfur CopperA
Type S (seamless pipe)
Grade A 0.25 0.95 0.05 0.045 0.40 0.40 0.40 0.15 0.08
Grade B 0.30 1.20 0.05 0.045 0.40 0.40 0.40 0.15 0.08
Type E (electric-resistance-welded)
Grade A 0.25 0.95 0.05 0.045 0.40 0.40 0.40 0.15 0.08
Grade B 0.30 1.20 0.05 0.045 0.40 0.40 0.40 0.15 0.08
Type F (furnace-welded pipe)
or basic oxygen
Grade A 0.30 1.20 0.05 0.045 0.40 0.40 0.40 0.15 0.08
The combination of these ﬁve elements shall not exceed 1.00 %.
TABLE 2 Tensile Requirements
Type F Types E and S
Grade A Grade B
Tensile strength, min, psi
48 000  48 000  60 000 
Yield strength, min, psi,
30 000  30 000  35 000 
Elongation in 2 in. [50 mm] A,B A,B A,B
The minimum elongation in 2 in. [50 mm] shall be that determined by the
e 5 625 000 @1940# A0.2
e = minimum elongation in 2 in. [50 mm] in percent rounded to the nearest
A = cross-sectional area of the tension specimen, rounded to the nearest
], based on the speciﬁed outside diameter or the nominal
specimen width and speciﬁed wall thickness. If the area calculated is
equal to or greater than 0.75 in.2
], then the value 0.75 in.2
] shall be used, and
U = speciﬁed tensile strength, psi [MPa].
See Table X4.1 or Table X4.2, whichever is applicable, for minimum elongation
values for various size tension specimens and grades.
A 53/A 53M
3.1.14 Selection of applicable level of preservation and
packaging and level of packing required, if other than as
speciﬁed or if MIL-STD-163 applies (see 21.2).
4. Materials and Manufacture
4.1 The steel for both seamless and welded pipe shall be
made by one or more of the following processes: open-hearth,
electric-furnace, or basic-oxygen.
4.2 When steels of different grades are sequentially strand
cast, identiﬁcation of the resultant transition material is re-
quired. The producer shall remove the transition material by
any established procedure that positively separates the grades.
4.3 The weld seam of electric-resistance welded pipe in
Grade B shall be heat treated after welding to a minimum of
1000°F [540°C] so that no untempered martensite remains, or
otherwise processed in such a manner that no untempered
4.4 When pipe is cold expanded, the amount of expansion
shall not exceed 11⁄2 % of the outside diameter pipe size.
5. Chemical Composition
5.1 The steel shall conform to the requirements as to
chemical composition in Table 1 and the chemical analysis
shall be in accordance with Test Methods, Practices, and
Terminology A 751.
6. Product Analysis
6.1 The purchaser is permitted to perform an analysis of two
pipes from each lot of 500 lengths, or fraction thereof. Samples
for chemical analysis, except for spectrographic analysis, shall
be taken in accordance with Method E 59. The chemical
composition thus determined shall conform to the requirements
speciﬁed in Table 1.
6.2 If the analysis of either pipe does not conform to the
requirements speciﬁed in Table 1, analyses shall be made on
additional pipes of double the original number from the same
lot, each of which shall conform to the requirements speciﬁed.
7. Tensile Requirements
7.1 The material shall conform to the requirements as to
tensile properties prescribed in Table 2.
7.2 The yield strength corresponding to a permanent offset
of 0.2 % of the gage length of the specimen or to a total
extension of 0.5 % of the gage length under load shall be
7.3 The test specimen taken across the weld shall show a
tensile strength not less than the minimum tensile strength
speciﬁed for the grade of pipe ordered. This test will not be
required for pipe under NPS 8 [DN 200].
7.4 Transverse tension test specimens for electric-welded
pipe NPS 8 [DN 200] and larger shall be taken opposite the
weld. All transverse test specimens shall be approximately 11⁄2
in. [40 mm] wide in the gage length, and shall represent the full
wall thickness of the pipe from which the specimen was cut.
This test is required for NPS 8 [DN 200] and larger.
8. Bending Requirements
8.1 For pipe NPS 2 [DN 50] and under, a sufficient length of
pipe shall be capable of being bent cold through 90° around a
cylindrical mandrel, the diameter of which is twelve times the
outside diameter of the pipe, without developing cracks at any
portion and without opening the weld.
8.2 When ordered for close coiling, the pipe shall stand
being bent cold through 180° around a cylindrical mandrel, the
diameter of which is eight times the outside diameter of the
pipe, without failure.
8.3 Double-extra-strong pipe over NPS 11⁄4 [DN 32] need
not be subjected to the bend test.
9. Flattening Test
9.1 The ﬂattening test shall be made on pipe over NPS 2
[DN 50] with all thicknesses extra strong and lighter.
9.2 Seamless Pipe:
9.2.1 For seamless pipe, a test specimen at least 2 1⁄2 in. [60
mm] in length shall be ﬂattened cold between parallel plates in
two steps. During the ﬁrst step, which is a test for ductility, no
cracks or breaks on the inside, outside, or end surfaces, except
as provided for in 9.7, shall occur until the distance between
the plates is less than the value of H calculated as follows:
H 5 ~1 1e!t/~e 1 t/D!
H = distance between ﬂattening plates, in. [mm] (Note 4),
e = deformation per unit length (constant for a
given grade of steel, 0.09 for Grade A, and 0.07
for Grade B),
t = nominal wall thickness, in. [mm], and
D = speciﬁed outside diameter, in. [mm]
9.2.2 During the second step, which is a test for soundness,
the ﬂattening shall be continued until the test specimen breaks
or the opposite sides of the pipe meet. Evidence of laminated
or unsound material that is revealed during the entire ﬂattening
test shall be cause for rejection.
NOTE 4—The H values have been calculated for standard and extra-
heavy weight sizes from NPS 21⁄2 to NPS 24 [DN 65 to DN 600],
inclusive, and are shown in Table X2.1.
9.3 Electric-Resistance-Welded Pipe— A test specimen at
least 4 in. [100 mm] in length shall be ﬂattened cold between
parallel plates in three steps, with the weld located either 0° or
90° from the line of direction of force as required in 9.3.1 or
9.3.2, whichever is applicable. During the ﬁrst step, which is a
test for ductility of the weld, no cracks or breaks on the inside
or outside surfaces shall occur until the distance between the
plates is less than two thirds of the original outside diameter of
the pipe. As a second step, the ﬂattening shall be continued.
During the second step, which is a test for ductility exclusive
of the weld, no cracks or breaks on the inside or outside
surfaces, except as provided for in 9.7, shall occur until the
distance between the plates is less than one third of the original
outside diameter of the pipe but is not less than ﬁve times the
wall thickness of the pipe. During the third step, which is a test
for soundness, the ﬂattening shall be continued until the test
specimen breaks or the opposite walls of the pipe meet.
Evidence of laminated or unsound material or of incomplete
weld that is revealed during the entire ﬂattening test shall be
cause for rejection.
9.3.1 For pipe produced in single lengths, the ﬂattening test
speciﬁed in 9.3 shall be made using a test specimen taken from
A 53/A 53M
each end of each length of pipe. The tests from each end shall
be made alternately with the weld at 0° and at 90° from the line
of direction of force.
9.3.2 For pipe produced in multiple lengths, the ﬂattening
test speciﬁed in 9.3 shall be made as follows:
126.96.36.199 Test specimens taken from, and representative of,
the front end of the ﬁrst pipe intended to be supplied from each
coil, the back end of the last pipe intended to be supplied from
each coil, and each side of any intermediate weld stop location
shall be ﬂattened with the weld located at 90° from the line of
direction of force.
188.8.131.52 Test specimens taken from pipe at any two locations
intermediate to the front end of the ﬁrst pipe and the back end
of the last pipe intended to be supplied from each coil shall be
ﬂattened with the weld located at 0° from the line of direction
9.3.3 For pipe that is to be subsequently reheated through-
out its cross section and hot formed by a reducing process, the
manufacturer shall have the option of obtaining the ﬂattening
test specimens required by 9.3.1 or 9.3.2, whichever is appli-
cable, either prior to or after such hot reducing.
9.4 Continuous-Welded Pipe—For continuous-welded pipe,
a specimen not less than 4 in. [100 mm] in length shall be
ﬂattened cold between parallel plates in three steps. The weld
shall be located 90° from the line of direction of force. During
the ﬁrst step, which is a test for quality of the weld, no cracks
or breaks on the inside, outside, or end surfaces shall occur
until the distance between the plates is less than three fourths
of the original outside diameter for butt-welded pipe. As a
second step, the ﬂattening shall be continued. During the
second step, which is a test for ductility exclusive of the weld,
no cracks or breaks on the inside, outside, or end surfaces,
except as provided for in 9.7, shall occur until the distance
between the plates is less than 60 % of the original outside
diameter for continuous-welded pipe. During the third step,
which is a test for soundness, the ﬂattening shall be continued
until the specimen breaks or the opposite walls of the pipe
meet. Evidence of laminated or unsound material or of incom-
plete weld that is revealed during the entire ﬂattening test shall
be cause for rejection.
9.5 Surface imperfections in the test specimen before ﬂat-
tening, but revealed during the ﬁrst step of the ﬂattening test,
shall be judged in accordance with the ﬁnish requirements in
9.6 Superﬁcial ruptures as a result of surface imperfections
shall not be cause for rejection.
9.7 When low D-to- t ratio tubulars are tested, because the
strain imposed due to geometry is unreasonably high on the
inside surface at the 6 and 12 o’clock locations, cracks at these
locations shall not be cause for rejection if the D-to-t ratio is
less than 10.
10. Hydrostatic Test
10.1 The hydrostatic test shall be applied, without leakage
through the pipe wall, to each length of pipe except as provided
in 11.2 for seamless pipe.
10.2 Each length of plain-end pipe shall be hydrostatically
tested to the pressures prescribed in Table X2.2, and each
threaded-and-coupled length shall be hydrostatically tested to
the pressures prescribed in Table X2.3. It shall be permissible,
at the discretion of the manufacturer, to perform the hydrostatic
test on pipe with plain ends, with threads only, or with threads
and couplings and also shall be permissible to test pipe in either
single lengths or multiple lengths.
NOTE 5—The hydrostatic test pressures given herein are inspection test
pressures, are not intended as a basis for design, and do not have any direct
relationship to working pressures.
10.3 The minimum hydrostatic test pressure required to
satisfy these requirements need not exceed 2500 psi [17 200
kPa] for NPS 3 [DN 80] and under, nor 2800 psi [19 300 kPa]
for all sized over NPS 3 [DN 80]. This does not prohibit testing
at a higher pressure at the manufacturer’s option. The hydro-
static pressure shall be maintained for not less than 5 s for all
sizes of seamless and electric-welded pipe.
11. Nondestructive Electric Test
11.1 Type E Pipe:
11.1.1 The weld seam of each length of ERW pipe NPS 2
[DN 50] and larger shall be tested with a nondestructive
electric test as follows:
11.1.2 Ultrasonic and Electromagnetic Inspection—Any
equipment utilizing the ultrasonic or electromagnetic principles
and capable of continuous and uninterrupted inspection of the
weld seam shall be used. The equipment shall be checked with
an applicable reference standard as described in 11.1.3 at least
once every working turn or not more than 8 h to demonstrate
its effectiveness and the inspection procedures. The equipment
shall be adjusted to produce well-deﬁned indications when the
reference standard is scanned by the inspection unit in a
manner simulating the inspection of the product.
11.1.3 Reference Standards—The length of the reference
standards shall be determined by the pipe manufacturer, and
they shall have the same speciﬁed diameter and thickness as
the product being inspected. Reference standards shall contain
machined notches, one on the inside surface and one on the
outside surface, or a drilled hole, as shown in Fig. 1, at the
option of the pipe manufacturer. The notches shall be parallel
to the weld seam, and shall be separated by a distance sufficient
to produce two separate and distinguishable signals. The 1⁄8-in.
[3.2-mm] hole shall be drilled through the wall and perpen-
dicular to the surface of the reference standard as shown in Fig.
1. Care shall be taken in the preparation of the reference
standard to ensure freedom from ﬁns or other edge roughness,
or distortion of the pipe.
NOTE 6—The calibration standards deﬁned in 11.1.3 are convenient
standards for calibration of nondestructive testing equipment. The dimen-
sions of such standards are not to be construed as the minimum sizes of
imperfections detectable by such equipment.
11.1.4 Acceptance Limits—Table 3 gives the height of
acceptance limit signals in percent of the height of signals
produced by reference standards. Imperfections in the weld
seam that produce a signal greater than the acceptance limit
signal given in Table 3 shall be considered a defect unless the
pipe manufacturer can demonstrate that the imperfection does
not reduce the effective wall thickness beyond 121⁄2 % of the
speciﬁed wall thickness.
11.2 Seamless Pipe—As an alternative to the hydrostatic
A 53/A 53M
test, and when speciﬁed by the purchaser, the full body of each
seamless pipe shall be tested with a nondestructive electric test
in accordance with Practices E 213, E 309, or E 570. In this
case each length so furnished shall include the mandatory
marking of the letters “NDE.” Except as provided in 184.108.40.206 it
is the intent of this test to reject pipe with imperfections which
produce test signals equal to or greater than that of the
11.2.1 When the nondestructive electric test is performed,
the lengths shall be marked with the letters “NDE.” The
certiﬁcation, when required, shall state Nondestructive Electric
Tested and shall indicate which of the tests was applied. Also,
the letters NDE shall be appended to the product speciﬁcation
number and material grade shown on the certiﬁcation.
11.2.2 The following information is intended to facilitate
the use of this speciﬁcation.
220.127.116.11 The calibration standards deﬁned in 11.2.3 through
11.2.5 are convenient standards for calibration of nondestruc-
tive testing equipment. The dimensions of such standards are
not to be construed as the minimum sizes of imperfections
detectable by such equipment.
18.104.22.168 The ultrasonic testing referred to in this speciﬁca-
tion is capable of detecting the presence and location of
signiﬁcant longitudinally or circumferentially oriented imper-
fections; however, different techniques need to be employed
for the detection of differently oriented imperfections. Ultra-
sonic testing is not necessarily capable of detecting short, deep
22.214.171.124 The eddy current examination referenced in this
speciﬁcation has the capability of detecting signiﬁcant discon-
tinuities, especially of the short abrupt type.
126.96.36.199 The ﬂux leakage examination referred to in this
speciﬁcation is capable of detecting the presence and location
of signiﬁcant longitudinally or transversely oriented disconti-
nuities. The provisions of this speciﬁcation only require
longitudinal calibration for ﬂux leakage. Different techniques
need to be employed for the detection of differently oriented
188.8.131.52 The hydrostatic test referred to in 10.2 has the
capability of ﬁnding imperfections of a size permitting the test
ﬂuid to leak through the tube wall and may be either visually
seen or detected by a loss of pressure. Hydrostatic testing is not
necessarily capable of detecting very tight through-the-wall
imperfections or imperfections that extend an appreciable
distance into the wall without complete penetration.
184.108.40.206 A purchaser interested in ascertaining the nature
(type, size, location, and orientation) of imperfections that are
capable of being detected in the speciﬁc application of these
examinations is directed to discuss this with the manufacturer
of the tubular product.
11.2.3 For ultrasonic testing, the calibration reference
notches shall be at the option of the producer, and shall be any
one of the three common notch shapes shown in Practice
E 213. The depth of notch shall not exceed 12.5 % of the
speciﬁed wall thickness of the pipe or 0.004 in. [0.1 mm],
whichever is greater.
11.2.4 For eddy current testing, the calibration pipe shall
contain, at the option of the producer, any one of the following
calibration standards to establish a minimum sensitivity level
220.127.116.11 Drilled Hole—Depending upon the pipe diameter
the calibration pipe shall contain three holes spaced 120° apart
or four holes spaced 90° apart and sufficiently separated
FIG. 1 Calibration Standards
TABLE 3 Acceptance Limits
Type Notch Size of Hole Acceptance
Signal, %in. mm
A 53/A 53M
longitudinally to ensure separately distinguishable responses.
The holes shall be drilled radially and completely through the
pipe wall, care being taken to avoid distortion of the pipe while
drilling. Depending upon the pipe diameter the calibration pipe
shall contain the following hole:
NPS DN Diameter of Drilled Hole
# 1⁄2 # 15 0.039 in. [1 mm]
> 1⁄2 # 11⁄4 > 15 # 32 0.055 in. [1.4 mm]
> 11⁄4 # 2 > 32 # 50 0.071 in. [1.8 mm]
> 2 # 5 > 50 # 125 0.087 in. [2.2 mm]
> 5 > 125 0.106 in. [2.7 mm]
18.104.22.168 Transverse Tangential Notch—Using a round tool
or ﬁle with a 1⁄4 in. [6 mm] diameter, a notch shall be ﬁled or
milled tangential to the surface and transverse to the longitu-
dinal axis of the pipe. The notch shall have a depth not
exceeding 12.5 % of the speciﬁed wall thickness of the pipe or
0.012 in. [0.3 mm], whichever is greater.
22.214.171.124 Longitudinal Notch—A notch 0.031 in. [0.8 mm]
or less in width shall be machined in a radial plane parallel to
the tube axis on the outside surface of the pipe, to have a depth
not exceeding 12.5 % of the speciﬁed wall thickness of the tube
or 0.012 in. [0.3 mm], whichever is greater. The length of the
notch shall be compatible with the testing method.
126.96.36.199 Compatibility—The discontinuity in the calibration
pipe shall be compatible with the testing equipment and the
method being used.
11.2.5 For ﬂux leakage testing, the longitudinal calibration
reference notches shall be straight sided notches machined in a
radial plane parallel to the pipe axis. For wall thickness under
0.500 in. [12.7 mm], outside and inside notches shall be used.
For wall thickness equal and above 0.500 in. [12.7 mm], only
an outside notch shall be used. Notch depth shall not exceed
12.5 % of the speciﬁed wall thickness, or 0.012 in. [0.3 mm],
whichever is greater. Notch length shall not exceed 1 in. [25
mm], and the width shall not exceed the depth. Outside
diameter and inside diameter notches shall be located suffi-
ciently apart to allow separation and identiﬁcation of the
11.2.6 Pipe containing one or more imperfections that
produce a signal equal to or greater than the signal produced by
the calibration standard shall be rejected or the area producing
the signal shall be rejected.
188.8.131.52 Test signals produced by imperfections that cannot
be identiﬁed, or produced by cracks or crack-like imperfec-
tions, shall result in rejection of the pipe, unless it is repaired
and retested. To be accepted, the pipe must pass the same
speciﬁcation test to which it was originally subjected, provided
that the remaining wall thickness is not decreased below that
permitted by the speciﬁcation. It shall be permissible to reduce
the outside diameter at the point of grinding by the amount so
184.108.40.206 It shall be permissible to evaluate test signals
produced by visual imperfections in accordance with provi-
sions of Section 14. A few examples of these imperfections
would be straightener marks, cutting chips, scratches, steel die
stamps, stop marks, or pipe reducer ripple.
11.2.7 The test methods described in this section are not
necessarily capable of inspecting the end portion of pipes. This
condition is referred to as end effect. The length of the end
effect shall be determined by the manufacturer and, when
speciﬁed in the purchase order, reported to the purchaser.
12. Permissible Variations in Weight and Dimensions
12.1 Weight—The weight of the pipe as speciﬁed in Table
X2.2 and Table X2.3 or as calculated from the relevant
equation in ASME B36.10M shall not vary by more than
NOTE 7—The weight tolerance is determined from the weights of the
customary lifts of pipe as produced for shipment by the mill, divided by
the number of feet of pipe in the lift. On pipe sizes over NPS 4 [DN 100],
where individual lengths are weighed, the weight tolerance is applicable to
the individual length.
12.2 Diameter—For pipe NPS 11⁄2 [DN 40] and under, the
outside diameter at any point shall not vary more than 6 1⁄64 in.
[0.4 mm] from the standard speciﬁed. For pipe NPS 2 [DN 50]
and over, the outside diameter shall not vary more than 61 %
from the standard speciﬁed.
12.3 Thickness—The minimum wall thickness at any point
shall be not more than 12.5 % under the nominal wall thickness
speciﬁed. The minimum wall thickness on inspection shall
conform to the requirements in Table X2.4.
13. End Finish
13.1 When ordered with plain ends, the pipe shall be
furnished to the following practice, unless otherwise speciﬁed.
13.1.1 NPS 11⁄2 [DN 40] and Smaller—Unless otherwise
speciﬁed on the purchase order, end ﬁnish shall be at the option
of the manufacturer.
13.1.2 NPS 2 [DN 50] and Larger:
220.127.116.11 Pipe of standard or extra strong weights, or in wall
thickness less than 0.500 in. [12.7 mm], other than double extra
strong pipe, shall be plain-end beveled with ends beveled to an
angle of 30°, +5°, −0°, measured from a line drawn perpen-
dicular to the axis of the pipe, and with a root face of 1⁄16 in. 6
1⁄32 in. [1.6 mm 6 0.8 mm].
18.104.22.168 Pipe with wall thicknesses over 0.500 in. [12.7
mm], and all double extra strong, shall be plain-end square cut.
13.2 When ordered with threaded ends, the pipe ends shall
be provided with a thread in accordance with the gaging
practice and tolerances of ANSI B1.20.1. For standard-weight
pipe NPS 6 [DN 150] and smaller, refer to Table X3.1 for
threading data. For standard-weight pipe NPS 8 [DN 200] and
larger and all sizes of extra-strong weight and double extra-
strong weight, refer to Table X3.2 for threading data. Threaded
pipe NPS 4 [DN 100] and larger shall have thread protectors on
the ends not protected by a coupling.
13.3 When ordered with couplings, one end of each length
of pipe shall be provided with a coupling manufactured in
accordance with Speciﬁcation A 865. The coupling threads
shall be in accordance with the gaging practice of ANSI
B1.20.1. The coupling shall be applied handling-tight, unless
power-tight is speciﬁed on the order. Couplings are to be made
of steel. Taper-tapped couplings shall be furnished on all
weights of threaded pipe sizes NPS 21⁄2 [DN 65] and larger. For
pipe NPS 2 [DN 50] and smaller, it is regular practice to
furnish straight-tapped couplings for standard-weight pipe and
taper-tapped couplings for extra-strong and double extra-strong
pipe. If taper-tapped couplings are required for pipe NPS 2
A 53/A 53M
[DN 50] and smaller on standard-weight pipe, it is recom-
mended that line pipe threads in accordance with API Speci-
ﬁcation 5L be ordered. The taper-tapped couplings provided on
line pipe in these sizes may be used on mill-threaded standard-
weight pipe of the same size.
14. Workmanship, Finish and Appearance
14.1 The pipe manufacturer shall explore a sufficient num-
ber of visual surface imperfections to provide reasonable
assurance that they have been properly evaluated with respect
14.2 Surface imperfections that penetrate more than 121⁄2 %
of the nominal wall thickness or encroach on the minimum
wall thickness shall be considered defects. Pipe with defects
shall be given one of the following dispositions:
14.2.1 The defect shall be removed by grinding, provided
that the remaining wall thickness is within speciﬁed limits,
14.2.2 Type S pipe and the parent metal of Type E pipe,
except within 1⁄2 in. [13 mm] of the fusion line of the electric
resistance seam, are permitted to be repaired in accordance
with the welding provisions of 14.5. Repair welding of Type F
pipe and the weld seam of Type E is prohibited.
14.2.3 The section of pipe containing the defect may be cut
off within the limits of requirement on length, or
14.3 At the purchaser’s discretion, pipe shall be subjected to
rejection if surface defects repaired in accordance with 14.2 are
not scattered, but appear over a large area in excess of what is
considered a workmanlike ﬁnish. Disposition of such pipe shall
be a matter of agreement between the manufacturer and the
14.4 When imperfections or defects are removed by grind-
ing, a smooth curved surface shall be maintained, and the wall
thickness shall not be decreased below that permitted by this
speciﬁcation. It shall be permissible to reduce the outside
diameter at the point of grinding by the amount so removed.
14.4.1 Wall thickness measurements shall be made with a
mechanical caliper or with a properly calibrated nondestruc-
tive testing device of appropriate accuracy. In the case of a
dispute, the measurement determined by use of the mechanical
caliper shall govern.
14.5 Weld repair shall be permitted only subject to approval
of the purchaser and in accordance with Speciﬁcation A 530/
14.6 The ﬁnished pipe shall be reasonably straight.
14.7 The pipe shall contain no dents greater than 10 % of
the pipe diameter or 1⁄4 in. [6 mm], whichever is smaller,
measured as a gap between the lowest point of the dent and a
prolongation of the original contour of the pipe. Cold-formed
dents deeper than 1⁄8 in. [3 mm] shall be free of sharp bottom
gouges; it shall be permissible to remove the gouges by
grinding, provided that the remaining wall thickness is within
speciﬁed limits. The length of the dent in any direction shall
not exceed one half the pipe diameter.
15. Number of Tests
15.1 Except as required by 15.2, one of each of the tests
speciﬁed in Section 7, 8.2, and Section 9 shall be made on test
specimens taken from one length of pipe from each lot of each
pipe size. For continuous-welded pipe, a lot shall contain no
more than 25 tons [23 Mg] of pipe for pipe sizes NPS 11⁄2 [DN
40] and smaller, and no more than 50 tons [45 Mg] of pipe for
pipe sizes NPS 2 [DN 50] and larger. For seamless and
electric-resistance-welded pipe, a lot shall contain no more
than one heat, and at the option of the manufacturer shall
contain no more than 500 lengths of pipe (as initially cut after
the ﬁnal pipe-forming operation, prior to any further cutting to
the required ordered lengths) or 50 tons [45 Mg] of pipe.
15.2 The number of ﬂattening tests for electric-resistance-
welded pipe shall be in accordance with 9.3.1 or 9.3.2,
whichever is applicable.
15.3 Except as allowed by 11.2, each length of pipe shall be
subjected to the hydrostatic test speciﬁed in Section 10.
16.1 If the results of the mechanical tests of any lot do not
conform to the requirements speciﬁed in Sections 7, 8, and 9,
retests are permitted to be made on additional pipe of double
the original number from the same lot, each of which shall
conform to the requirements speciﬁed.
16.2 For pipe produced in single lengths, if any section of
the pipe fails to comply with the requirements of 9.3, it shall be
permissible to cut other sections from the same end of the same
length until satisfactory tests are obtained, except that the
ﬁnished pipe shall not be shorter than 80 % of its length after
the original cropping; otherwise the length shall be rejected.
For pipe produced in multiple lengths, it shall be permissible to
cut retests from each end of each individual length in the
multiple. Such tests shall be made with the weld alternately 0°
and 90° from the line of direction of force.
17. Test Methods
17.1 The test specimens and the tests required by this
speciﬁcation shall conform to those described in the latest issue
of Test Methods and Deﬁnitions A 370.
17.2 The longitudinal tension test specimen shall be taken
from the end of the pipe or, for continuous-welded pipe, it shall
be permissible to be taken from the skelp, at a point approxi-
mately 90° from the weld, and shall not be ﬂattened between
gage marks. The sides of each specimen shall be parallel
between gage marks. If desired, the tension tests are permitted
to be made on the full section of pipe. When impracticable to
pull a test specimen in full section, the standard 2-in. [50-mm]
gage length tension test specimen shown in Fig. A2.3 of Test
Methods and Deﬁnitions A 370 is acceptable.
17.3 Transverse weld test specimens from electric-
resistance-welded pipe shall be taken with the weld at the
center of the specimen. All transverse test specimens shall be
approximately 11⁄2 in. [40 mm] wide in the gage length and
shall represent the full wall thickness of the pipe from which
the specimen was cut.
17.4 Test specimens for the bend and ﬂattening tests shall be
taken from pipe. Test specimens for the ﬂattening test shall be
smooth on the ends and free from burrs.
17.5 All specimens shall be tested at room temperature.
18.1 Unless otherwise speciﬁed, pipe lengths shall be in
A 53/A 53M
accordance with the following regular practice.
18.1.1 Pipe of weights lighter than extra strong shall be in
single-random lengths of 16 to 22 ft [4.88 to 6.71 m], but not
more than 5 % of the total number of threaded lengths are
permitted to be jointers (two pieces coupled together). When
ordered with plain ends, 5 % are permitted to be in lengths of
12 to 16 ft [3.66 to 4.88 m].
18.1.2 Pipe of extra-strong and heavier weights shall be in
random lengths of 12 to 22 ft [3.66 to 6.71 m]. Five percent are
permitted to be in lengths of 6 to 12 ft [1.83 to 3.66 m].
18.1.3 When extra-strong or lighter pipe is ordered in
double-random lengths, the minimum lengths shall be not less
than 22 ft [6.71 m], with a minimum average for the order of
35 ft [10.67 m].
18.1.4 When lengths longer than single random are required
for wall thicknesses heavier than extra-strong, the length shall
be subject to negotiation.
18.1.5 When pipe is furnished with threads and couplings,
the length shall be measured to the outer face of the coupling.
19. Galvanized Pipe
19.1 Galvanized pipe ordered under this speciﬁcation shall
be coated with zinc inside and outside by the hot-dip process.
The zinc used for the coating shall be any grade of zinc
conforming to Speciﬁcation B 6.
19.2 Weight of Coating—The weight of zinc coating shall
be not less than 1.8 oz/ft2
[0.55 kg/m 2
] as determined from the
average results of the two specimens taken for test in the
manner prescribed in 19.5 and not less than 1.6 oz/ft2
] for either of these specimens. The weight of coating
expressed in ounces per square foot shall be calculated by
dividing the total weight of zinc, inside plus outside, by the
total area, inside plus outside, of the surface coated. Each
specimen shall have not less than 1.3 oz/ft2
zinc coating on each surface, calculated by dividing the total
weight of zinc on the given surface (outside or inside) by the
area of the surface coated (outside or inside).
19.3 Weight of Coating Test—The weight of zinc coating
shall be determined by a stripping test in accordance with Test
Method A 90. The total zinc on each specimen shall be
determined in a single stripping operation.
19.4 Test Specimens—Test specimens for determination of
weight of coating shall be cut approximately 4 in. [100 mm] in
19.5 Number of Tests—Two test specimens for the determi-
nation of weight of coating shall be taken, one from each end
of one length of galvanized pipe selected at random from each
lot of 500 lengths or fraction thereof, of each size.
19.6 Retests—If the weight of coating of any lot does not
conform to the requirements speciﬁed in 19.2, retests of two
additional pipes from the same lot shall be made, each of which
shall conform to the requirements speciﬁed.
19.7 When pipe ordered under this speciﬁcation is to be
galvanized, the tension, ﬂattening, and bend tests shall be made
on the base material before galvanizing. When speciﬁed,
results of the mechanical tests on the base material shall be
reported to the purchaser. If it is impracticable to make the
mechanical tests on the base material before galvanizing, it
shall be permissible to make such tests on galvanized samples,
and any ﬂaking or cracking of the zinc coating shall not be
considered cause for rejection. When galvanized pipe is bent or
otherwise fabricated to a degree that causes the zinc coating to
stretch or compress beyond the limit of elasticity, some ﬂaking
of the coating is acceptable.
20.1 The inspector representing the purchaser shall have
entry, at all times while work on the contract of the purchaser
is being performed, to all parts of the manufacturer’s works
that concern the manufacture of the material ordered. The
manufacturer shall afford the inspector all reasonable facilities
to satisfy him that the material is being furnished in accordance
with this speciﬁcation. All tests (except product analysis) and
inspection shall be made at the place of manufacture prior to
shipment, unless otherwise speciﬁed, and shall be so conducted
as not to interfere unnecessarily with the operation of the
21.1 The purchaser is permitted to inspect each length of
pipe received from the manufacturer and, if it does not meet the
requirements of this speciﬁcation based on the inspection and
test method as outlined in the speciﬁcation, the length shall be
rejected and the manufacturer shall be notiﬁed. Disposition of
rejected pipe shall be a matter of agreement between the
manufacturer and the purchaser.
21.2 Pipe found in fabrication or in installation to be
unsuitable for the intended use, under the scope and require-
ments of this speciﬁcation, shall be set aside and the manufac-
turer notiﬁed. Such pipe shall be subject to mutual investiga-
tion as to the nature and severity of the deﬁciency and the
forming or installation, or both, conditions involved. Disposi-
tion shall be a matter for agreement.
22.1 The producer or supplier shall, upon request, furnish to
the purchaser a certiﬁcate of inspection stating that the material
has been manufactured, sampled, tested, and inspected in
accordance with this speciﬁcation (including year of issue),
and has been found to meet the requirements.
22.2 Report—For Types E and S, the producer or supplier
shall furnish to the purchaser a chemical analysis report for the
elements speciﬁed in Table 1.
22.3 EDI—A certiﬁcate of inspection or chemical analysis
report printed from or used in electronic form from an
electronic data interchange (EDI) transmission shall be re-
garded as having the same validity as a counterpart printed in
the certiﬁer’s facility. The use and format of the EDI document
are subject to agreement between the purchaser and the
NOTE 8—EDI is the computer to computer exchange of business
information in a standard format such as ANSI ASC X12.
22.4 Notwithstanding the absence of a signature, the orga-
nization submitting the certiﬁcate of inspection or chemical
analysis report is responsible for its content.
23. Product Marking
23.1 Except as allowed by 23.5 and 23.6, each length of
A 53/A 53M
pipe shall be legibly marked in the following sequence by
rolling, stamping, or stenciling to show:
23.1.1 Manufacturer’s name or mark,
23.1.2 Speciﬁcation number (year of issue not required),
NOTE 9—Pipe that complies with multiple compatible speciﬁcations
may be marked with the appropriate designation for each speciﬁcation.
23.1.3 Size (NPS and weight class, schedule number, or
nominal wall thickness; or speciﬁed outside diameter and
nominal wall thickness),
23.1.4 Grade (A or B),
23.1.5 Type of pipe (F, E, or S),
23.1.6 Test pressure, seamless pipe only (if applicable, in
accordance with Table 4),
23.1.7 Nondestructive electric test, seamless pipe only (if
applicable, in accordance with Table 4),
23.2 Unless another marking format is speciﬁed in the
purchase order, length shall be marked in feet and tenths of a
foot, or metres to two decimal places, dependent upon the units
to which the pipe was ordered. The location of such marking
shall be at the option of the manufacturer.
23.3 Heat number, lot number, run number, or a combina-
tion thereof shall be marked at the option of the manufacturer,
unless speciﬁc marking is speciﬁed in the purchase order. The
location of such marking shall be at the option of the
23.4 Any additional information desired by the manufac-
turer or speciﬁed in the purchase order.
23.5 For pipe NPS 11⁄2 [DN 40] and smaller that is bundled,
it shall be permissible to mark this information on a tag
securely attached to each bundle.
23.6 When pipe sections are cut into shorter lengths by a
subsequent producer for resale as material, the processor shall
transfer complete identiﬁcation including the name or brand of
the manufacturer, to each unmarked cut length, or to metal tags
securely attached to unmarked pipe bundled in accordance with
the requirements of 23.5. The same material designation shall
be included with the information transferred, and the proces-
sor’s name, trademark, or brand shall be added.
23.7 Bar Coding—In addition to the requirements in 23.1,
23.5, and 23.6, bar coding is acceptable as a supplementary
identiﬁcation method. It is recommended that bar coding be
consistent with the Automotive Industry Action Group (AIAG)
standard prepared by the Primary Metals Subcommittee of the
AIAG Bar Code Project Team.
24. Government Procurement
24.1 When speciﬁed in the contract, material shall be
preserved, packaged, and packed in accordance with the
requirements of MIL-STD-163. The applicable levels shall be
as speciﬁed in the contract. Marking for shipment of such
material shall be in accordance with Fed. Std. No. 123 for civil
agencies and MIL-STD-129 or Federal Std. No. 183 if con-
tinuous marking is required, for military agencies.
24.2 Inspection—Unless otherwise speciﬁed in the contract,
the producer is responsible for the performance of all inspec-
tion and test requirements speciﬁed herein. Except as otherwise
speciﬁed in the contract, the manufacturer shall use its own or
any other suitable facilities for performing the inspection and
test requirements speciﬁed herein, unless otherwise disap-
proved by the purchaser in the contract or purchase order. The
purchaser shall have the right to perform any of the inspections
and tests set forth in this speciﬁcation where deemed necessary
to ensure that the material conforms to prescribed require-
25. Packaging and Package Marking
25.1 When speciﬁed on the purchase order, packaging,
marking, and loading or shipment shall be in accordance with
those procedures recommended by Practices A 700.
26.1 black steel pipe; seamless steel pipe; steel pipe; welded
steel pipe; zinc coated steel pipe
X1. DEFINITIONS OF TYPES OF PIPE
X1.1 Type F, Furnace-Butt-Welded Pipe, Continuous-
Welded—Pipe produced in continuous lengths from coiled
skelp and subsequently cut into individual lengths, having its
longitudinal butt joint forge welded by the mechanical pressure
developed in rolling the hot-formed skelp through a set of
round pass welding rolls.
X1.2 Type E, Electric-Resistance-Welded Pipe—Pipe pro-
duced in individual lengths or in continuous lengths from
coiled skelp and subsequently cut into individual lengths,
having a longitudinal butt joint wherein coalescence is pro-
duced by the heat obtained from resistance of the pipe to the
ﬂow of electric current in a circuit of which the pipe is a part,
and by the application of pressure.
X1.3 Type S, Wrought Steel Seamless Pipe—Wrought steel
seamless pipe is a tubular product made without a welded
seam. It is manufactured by hot working steel and, if necessary,
by subsequently cold ﬁnishing the hot-worked tubular product
to produce the desired shape, dimensions, and properties.
TABLE 4 Marking of Seamless Pipe
Hydro NDE Marking
Yes No Test pressure
No Yes NDE
Yes Yes Test Pressure/NDE
A 53/A 53M
The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection
with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such
patent rights, and the risk of infringement of such rights, are entirely their own responsibility.
This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and
if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards
and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible
technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your
views known to the ASTM Committee on Standards, at the address shown below.
This standard is copyrighted by ASTM, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.
Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at
610-832-9585 (phone), 610-832-9555 (fax), or email@example.com (e-mail); or through the ASTM website (www.astm.org).
A 53/A 53M